Journal of Mechanical Science and Engineering
Journal of Mechanical Science and Engineering Sriwijaya University was established in 2013
as online version.
Publication covering area of research and review papers are as follows but not limitted to:
Materials Engineering etc
Prof.Dr. DEA K Sahim, Mechanical Engineering Department Faculty of Engineering
Sriwijaya University, Indonesia
Mr. Irsyadi Yani, Mechanical Engineering Department, Indonesia
Dipl.-Ing. Ir. Amrifan Saladin Mohruni PhD., Mechanical Engineering Department
Faculty of Engineering Sriwijaya University, Indonesia
Dr. Agung - Mataram, Mechanical Engineering Department Faculty of Engineerig
Prof. Dr. Ir. Hasan Basri, Mechanical Engineering Department Faculty of Engineering
Sriwijaya University, Indonesia
Dr Diah Kusuma Pratiwi, Mechanical Engineering Department Faculty of Engineering
Sriwijaya Unviersity, Indonesia
Dr. Ir. Riman Sipahutar, MSc., Mechanical Engineering Department Faculty of
Engineering Sriwijaya University, Indonesia
Journal of Mechanical Science and Engineering Vol.1 No.1 October 2013 1
JOURNAL OF MECHANICAL
SCIENCE AND ENGINEERING
Vol.1 No.1 October 2013
The Carburizing Process of Low Carbon Steel
with Charcoal Media
Yahyaa,* Nukmanb Hendri Chandrab
Student of Master Program Mechanical Engineering, Sriwijaya University
Lecturer of Master Program Mechanical Engineering, Sriwijaya University
*Corresponding author: email@example.com
Received in revised form XXXX Accepted XXXX
Carburizing process is carried out to improve the power quality of a low carbon steel with a low cost. The material used is a type of low carbon steel with a carbon value of 0.25%. Carburizing process on low carbon steel at a temperature of 9000C with a holding time of 90 minutes using goat bone and coconut shell char medial. The use of goat bone charcoal carburizer produces higher hardness values of carbon steel with coconut shell charcoal media. Results of testing the value of carbon steel after carburizing processes with coconut shell was 0,423% whereas after carburizing process with goat bone carbon value of only 1,593%.
Keywords:carburizing process coconut shell, goat bone, hardness test, Tensile Test, Impact Test, and microstructure
© 2013 Journal of Mechanical Science and Engineering
Carburization is the process of adding the element carbon on the low carbon steel surface, carburizing heating carried out at the temperature 900oC until 950oC. Elemental carbon can be obtained from wood charcoal, coconut shell charcoal or materials that contain the element carbon. Carbonization aimed to providing more carbon content at the surface than carbon content at the inner wall, so that the surface hardness increases. Carburizing can be done in three ways, namely pack carburizing, liquid carburizing and gas carburizing. The use of goat bone charcoal and coconut shell in the pack carburizing is carried out at temperature 900°C and holding time 90 minutes.
Carburization is a way of hardening the surface of the metal which heating the metal above the surrounding critical temperature that contains carbon element. In critical temperature, carbon is absorbed into the metal and then become solid solution of
carbon-steel form which the outer layer contains high carbon content. At the suitable time, the carbon atoms will have the opportunity to difuse to inside layer. The layer thickness depends on temperature process and reaction time needed.
In the carburization process, steel that already in austenisasi put into an environment which contain high carbon content so that the carbon diffusion process on the surface can be done. Thus, there was a gradient of carbon content between the surface area and the core area. Diffusion process indicates two factors that can be used to control carburization. Absorption of carbon on the surface and diffusion of carbon in the metal can be used to determine the rate of carburization process.
The Carburizing Process of Low Carbon Steel with Charcoal Media 2
Advantages and disadvantages of the pack carburization process is as follows:
a. Advantages of carburization process is as follows:
• Can use variety of furnace because it does require a certain atmosphere.
• Efficiently and economically.
• Carburization media is easy to earn.
• Diffusion depth can be adjusted.
b. Disadvantages of carburization process is as
• Requires cleaning process of the surface
• Difficult to obtain the small depth because of the difficult controlling process.
• Difficult to control the carbon concentration in the surface area and carbon gradient as the gas carburization process.
• Not suitable for direct quenching process.
Pack carburization similar to gas carburization, that main gas sources at the surface of carburizing component are carbon monoxide. Voluntary carbon, absorbed by steel surface, form from decomposed carbon monoxide into carbon dioxide and voluntary carbon. Carbon dioxide will react directly with a solid solution to produce the new carbon monoxide form .
Steel can be defined as a mixture of carbon and iron, which carbon content (C) will affect the hardness of steel. The steel also contains other elements that are called alloys, alloying elements are phosphorus, sulfur, manganese, silicon. They acts as binds which the number of weight percent based on the standard uses and customized fabrication, which aims to improve the mechanical and physical properties. The physical properties is a natural properties that cannot be changed, For the example is the magnetic properties, metal density, electrically conductive and melting point. Low Carbon steel is one of carbon steel type, where the percentage of the element carbon below 0.25%C, to more clearly shown in Table 1, while the other forming elements such as Mn not more than 0.8%, Si is not more than 0.5%, while Cu element is not more than 0.6%. In addition, Types of carbon steel also grouped by the percentage composition of carbon alloying elements as shown in the phase diagram of Fe - C, steel hypoeutektoid contains less than 0.8% C, eutectoid steel contains 0.8%C, and hypereutectoid steel contains more than 0.8%C.
Table 1. Steel Classification based on Carbon Content
No Type of Carbon Steel Carbon Element (%)
1 Low Carbon Steel ≤0,25
2 Medium Carbon Steel 0,25 ÷ 0,55
3 High Carbon Steel > 0,55
Low carbon steel has physical and mechanical properties as follows:
a. Physical Properties
The physical properties of steel such as having good magnetic properties, high density metal, and high melting point (1600°C).
b. Mechanical Properties
Mechanical properties is a basic properties that can be changed and influenced by external factors. The effect of heating at a certain time and temperature, so that the metal microstructure change mechanical properties because of the warming. metal. Study about heat treatment in carburizing process had been done by several researchers  which concluded that the addition of elements (C) to the low-carbon steel resulted in the change of the maximum tensile strength owned by subsequent material. The changes in the value of the maximum tensile strength of low carbon steel showed an increase of pre-treatment and the experimental results in their research shows the average value of the maximum tensile strength is approximately 38%. The study of carburizing heat treatment has been investigated by any researchers  and concluded that the carburization process can reduce impact strengh of mild steel, but contrary to the trend observed that activated carbon is carburizer that increase the resilience impact and temperatur carburization. Bone powder is used as the carburizer in the process, so that the strength of mild steel will increase while carburizing process. But it will decrease while increasing temperature carburization. Carburization treatment is followed by cooling process of the oil at a temperature 550°C, greatly affect the hardness and the tensile strength of mild steel.
Carburization process will reduce the energy impact of the mild steel and then the strength
decreases while increasing carburization
temperature. The mechanical properties of mild steel are found to be highly influenced by the carburizing soaking temperature. Carburized sample is soaked for 15 minutes and the other is soaked at 900°C for 30 minutes and followed by oil cooling process. At temperature 550°C is considered the better condition because they showed a tendency hard surfaces with soft core. Study heat changes, especially about
carburization has been investigated by some
Journal of Mechanical Science and Engineering Vol.1 No.1 October 2013 3 carburization of sample which used palm kernel cell
powder, is involved at a temperature 1000°C until 1100°C. So that palm kernel shell and animal bone potentially to be used as mild steel carburizer, whereas lighter shells have a tendency to be used as a drop carburization.
The study of carburizing heat changing has been investigated by some researchers  concluded that the basic material (reinforced concrete KSTY) has
hardness (HV) - 915.77 N/mm2 after surface
hardening treatment process, using pack carburizing
until Quenching process obtained hardness
(HV) = 3178.45 N/mm2 with carbonization holding
time for three hours, or can be involved the increasing surface hardness about 46.22%. The Changing of carbon diffusion in iron KSTY is influenced by the treatment of carbonization process and carbonization resistant time. The percentage of changing surface hardness KSTY consists of one hour from standard until carburizing process involve the increasing of hardness 31.42%.
Figure 1. Flow Diagram of The Process
From the carbonization process until quenching process is 38.67% or an increasing average is 35.05%, then two hours of standard until the carburization process violence is increasing 38.67%. From the carburization process until quenching process is 45.47% or an increasing average is 41.17%, then three hours of standard until the
carburization process violence is increasing 41.06%. From the carburization process until quenching process is 51.38% or an increasing average 46.22%. The Carbonization process of Pack carburizing with a three-hour detention time and followed by quenching process is very suitable to increase the surface hardness of material power thresher (steel Making specimen
Carburization Process Temperature 900oC Holding Time 90 minute
Data of Testing Result
Coconut shell Charcoal Goat Bone
Tensile Strength Testing Making Charcoal
Carbon Content Testing
Micro Structure Testing Preparation
The Carburizing Process of Low Carbon Steel with Charcoal Media 4
concrete KSTY). Thus, the researchers were able to conclude that needed to be done further research investigated by researchers  that based on the results of the data studies can be concluded the
hardness changing from 212.18 kg/mm2 increase
until 257.5 kg/mm2 then obtained from impact
testing 0.350 Joule/mm2until 1.067 Joules/mm2.
2. METHOD AND PROCEDURE
From several journals literature that have been read, known that carburization process using goat bone charcoal has never done before. Therefore researcher is interested in conducting research using that media, and using coconut shell charcoal for comparative material in this study.
Flow diagram process has been made from
preparation of materials, making charcoal,
carburizing process, laboratory testing, data analysis and conclusions. And the benefit of this research such to knowing the changing of low carbon physical properties and mechanical properties due to the treatment of carburization process, and compare the carburization with goat bone charcoal media than carburization with coconut shell charcoal media.
Research methods in this study are followed by diagram as shown at Figure 1.
3. RESULTS AND DISCUSSION
Data analysis of the chemical composition goat bone charcoal and coconut shell, done at Chemical Engineering Laboratory Politeknik Sriwijaya on June 5th 2013 using Bomb Calori and Gravimetry apparatus, can be seen in Table 2 :
Table 2. The chemical composition of Goat Bone Charcoal and Coconut Shell Charcoal
2 Carbon, C 58.255 59.198
3 Abu 6.17 10.97
Data analysis of the chemical composition low carbon steel before carburization process, done at the Engineering Laboratory PT PUSRI Palembang, Sample Testing of Different Quality using Gra JISS G 3101 SS 400 on March 27th 2013, can be seen in the table below :
Table 3. Chemical composition of low carbon steel before carburizing process
Data analysis of the chemical composition low carbon steel after carburization process, done at the Engineering Laboratory PT PUSRI Palembang, Sample Testing of Different Quality using Gra JISS G 3101 SS 400 on March 27th 2013, can be seen in the table below :
Table 4. Chemical composition of low carbon steel after carburizing process
1 Fe 97.367 91.167
2 C 1.593 0.423
3 Si 0.025 1.75
4 Mn 0.606 1.27
5 Cr 0.112 0.376
6 Mo 0.0239 0.0948
7 Ni 0.0403 1.28
8 Al 0.0075 0.166
9 Co 0.0088 0.0458
10 Cu 0.148 2.59
11 Nb 0.0284 0.178
12 Ti 0.005 0.0698
13 V 0.0194 0.113
14 W 0.025 0.345
15 Pb 0.010 0.0458
Carburizing process has shown increasing hardness of low carbon steel material. With coconut shell charcoal composition for 59.198% (Table 2), the hardness can increase from 231.65 (kg/mm) to 262.85 (kg /mm). And with goat bone charcoal composition for 58.255% (Table 2), the hardness can increase from 347.63 (kg/mm) to 231.65 (kg/mm). Therefore goat bone charcoal more effective as a supplement in the carburizing process than coconut shell charcoal.
Graph of Vickers Hardness Testing, Low Carbon
Steel before carburizing, after carburizing
carburizing coconut shell charcoal and goat bone
charcoal done in the Mechanical engineering
Journal of Mechanical Science an Figure 2. Vickess Hardness Testin
Steel before and after Ca
Carburizing process has shown of low carbon steel material. W charcoal composition for 59.19 impact can decrease from 32 (Joule). And with goat bone ch for 58.255% (Table 2), the impac 32.3 (Joule) to 5.2 (Joule). Ther charcoal more effective as a carburizing process than goat bon
Graph of Impact Testing, L before carburizing, after carbur charcoal and goat bone charcoal 900oC and holding time 90 minute engineering laboratory Politekn Impact 450 Galdabini apparatus can be described as Figure 3 belo
and Engineering Vol.1 No.1 October 2013 esting of Low Carbon charcoal composition pact can decrease from herefore coconut shell a supplement in the bone charcoal.
, Low Carbon Steel urizing coconut shell al done at temperature nute in the Mechanical knik Sriwijaya using tus on May 31st 2013,
Figure 3. Impact Testing Before and After
Carburizing process has strength of low carbon ste shell charcoal compositio the tensile strength can (N/mm²) to 447.08 (N/mm charcoal composition for tensile strength can decre to 342.86 (N/mm²). Theref more effective as a supple process than goat bone cha
Graph of tensile strengt before carburizing, after charcoal and goat bone 900oC and holding time
Sriwijaya using Hung Ta T 2013, can be described as f
Figure 4. Tensile Strength Steel Before and
Photograph of micro str steel before and after car Mechanical Engineering la Using Olympus Microsco described as Figure 5 below
has shown decreasing tensile steel material. With coconut ition for 59.198% (Table 2), can decrease from 552.0 /mm²). And with goat bone for 58.255% (Table 2), the crease from 552.08 (N/mm²)
² refore coconut shell charcoal
pplement in the carburizing harcoal.
gth testing, low carbon steel r carburizing coconut shell ne charcoal at temperature e 90 minute done in the
ng laboratory Politeknik
a Type HT 9502 on June 1st s figure 4 below :
th Testing of Low Carbon nd After Carburizing
Figure 5. Micro Structure of low carbon Before carburization, Edge sec
charcoal (T = 900oC and HT =
coconut shell charcoal (T = carburization using goat bone c f. After carburization using goa 100 x
Based on the data analysis, the using o
charcoal and coconut shell charco
summarized as follows.
a. Goat bone charcoal as carburizing
increase the hardness of low c (347.63 kg/mm2) than using of c charcoal (262.85 kg/mm2). While u bone charcoal will decrease the tensile strength low carbon steel th the coconut shell charcoal.
b. Carbon content before carburizatio
0.25%, it means that the materials low carbon steel type. While after c process using coconut shell charcoa content of low carbon steel increas And after carburization process usin charcoal, the carbon content of low increase to 1.593%. Therefore content after carburization using
charcoal higher than using co
 A. Oyetunji and S.O. Adeosun.
Carburizing Process Variables on and Chemical Properties of Carb Steel. Journal of Basic and Applie 2012.
 Aramide F O.,Pack Carburiation o
using Pulverized Bone as Optimizing Process Parameters
Electronic Journal of Prac
Technologies.p. 1–12, 2010.
 Darmanto., Pengaruh Holding Time
Sifat Kekerasan dengan Refining Th Proses Carburizing Material B Rendah., Journal Mechanical Engin No.2, 2006.
Bidang pinggir dengan Arang Tempurung Kelapa
The Carburizing Proc
bon steel a. Before carburization, Middle section, Magn section, Magnification 100 x, c. After carburization u
= 90), Middle section, Magnification 200 x, d. After = 900oC and HT = 90), Edge section, Magnificatio
n of Mild Steel, s Carburizer:
 Kuswanto B., Peningkatan
Maksimum Material Baja Menggunakan Proses Pen Padat., Journal Mechanical No.3, 2010.
 Masyrukan.,Pengaruh Sifat
Baja Karbon Rendah Akiba Pengarbonan dari Arang K
Mechanical Engineering Vol.  Mujiono dan Arianto L
Efektifitas Karburisasi Padat Rendah dengan Optimasi Uk Tempurung Kelapa., Jou Engineering Vol.10 No.1, 200
 Mulyadi dan Eka S., K
Kekerasan dan Difusi Karb dari Proses Karburisasi dan pada Material Gigi Perontok
Journal Mechanical Engineer
 Siproni., Keefektifan Pengg
Arang Tulang Sapi pada Ba untuk Pembuatan Alat Pema Sawit (Dodos dan Egrek).,
Engineering Universitas Panc
rocess of Low Carbon Steel with Charcoal Media agnification 200 x, b.
using coconut shell ter carburization using tion 100 x, e. After Magnification 200 x, ection, Magnification
tan Kekuatan Tarik ja Karbon Rendah enambahan Karbon
al Engineering Vol.5
ifat Fisis Dan Mekanis bat Pengaruh Proses Kayu Jati., Journal ol.7 No.1, 2006.
dat pada Baja Karbon Ukuran Serbuk Arang